#------------------------------------------------------------------------------
#$Date: 2019-03-23 02:14:12 +0200 (Sat, 23 Mar 2019) $
#$Revision: 214297 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/04/94/7049414.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7049414
loop_
_publ_author_name
'Gui, Xin'
'Finkelstein, Gregory'
'Graf, David'
'Wei, Kaya'
'Zhang, Dongzhou'
'Baumbach, Ryan'
'Dera, Przemslaw'
'Xie, Weiwei'
_publ_section_title
;
 Enhanced Néel Temperature in EuSnP under Pressure
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/C9DT00449A
_journal_year                    2019
_chemical_formula_sum            'Eu P Sn'
_chemical_formula_weight         301.62
_chemical_name_systematic
;
 ?
;
_space_group_crystal_system      tetragonal
_space_group_IT_number           129
_space_group_name_Hall           '-P 4a 2a'
_space_group_name_H-M_alt        'P 4/n m m'
_symmetry_space_group_name_Hall  '-P 4a 2a'
_symmetry_space_group_name_H-M   'P 4/n m m :2'
_audit_creation_method           SHELXL-2013
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.2229(6)
_cell_length_b                   4.2229(6)
_cell_length_c                   8.6314(17)
_cell_measurement_reflns_used    703
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      38.971
_cell_measurement_theta_min      2.360
_cell_volume                     153.92(4)
_computing_cell_refinement       GSE_ADA/RSV
_computing_data_collection       GSE_ADA/RSV
_computing_data_reduction        GSE_ADA/RSV
_computing_molecular_graphics    GSE_ADA/RSV
_computing_publication_material  GSE_ADA/RSV
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.852
_diffrn_measured_fraction_theta_max 0.523
_diffrn_measurement_device_type  'synchrotron x-ray CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.4335
_diffrn_reflns_av_R_equivalents  0.0956
_diffrn_reflns_av_unetI/netI     0.0394
_diffrn_reflns_Laue_measured_fraction_full 0.852
_diffrn_reflns_Laue_measured_fraction_max 0.523
_diffrn_reflns_limit_h_max       2
_diffrn_reflns_limit_h_min       -3
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            703
_diffrn_reflns_point_group_measured_fraction_full 0.852
_diffrn_reflns_point_group_measured_fraction_max 0.523
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         38.971
_diffrn_reflns_theta_min         2.360
_exptl_absorpt_coefficient_mu    7.493
_exptl_absorpt_correction_type   none
_exptl_absorpt_process_details   None
_exptl_crystal_colour            Silver
_exptl_crystal_density_diffrn    6.508
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'Not measured'
_exptl_crystal_description       Plate
_exptl_crystal_F_000             256
_exptl_crystal_size_max          0.025
_exptl_crystal_size_mid          0.020
_exptl_crystal_size_min          0.015
_exptl_transmission_factor_max   0.7434
_exptl_transmission_factor_min   0.3457
_refine_diff_density_max         4.304
_refine_diff_density_min         -4.470
_refine_diff_density_rms         0.851
_refine_ls_extinction_coef       None
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.315
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     10
_refine_ls_number_reflns         161
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.315
_refine_ls_R_factor_all          0.0544
_refine_ls_R_factor_gt           0.0544
_refine_ls_shift/su_max          0.111
_refine_ls_shift/su_mean         0.010
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0556P)²+19.8607P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1666
_refine_ls_wR_factor_ref         0.1666
_reflns_Friedel_coverage         0.000
_reflns_number_gt                161
_reflns_number_total             161
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            c9dt00449a2.cif
_cod_data_source_block           EuSnP-p2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'None' changed to 'none'
according to
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

'_exptl_crystal_density_meas' value 'None' was changed to '?' - the
value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 4973 2017-02-22 13:04:09Z antanas 
;
_cod_original_cell_volume        153.92(5)
_cod_database_code               7049414
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelxl_version_number           2013-4
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, -y+1/2, z'
'-y+1/2, x, z'
'y, -x+1/2, z'
'-x, y+1/2, -z'
'x+1/2, -y, -z'
'y+1/2, x+1/2, -z'
'-y, -x, -z'
'-x, -y, -z'
'x-1/2, y-1/2, -z'
'y-1/2, -x, -z'
'-y, x-1/2, -z'
'x, -y-1/2, z'
'-x-1/2, y, z'
'-y-1/2, -x-1/2, z'
'y, x, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Eu1 Eu 0.2500 0.2500 0.6713(2) 0.0126(8) Uani 1 8 d S T P
Sn2 Sn 0.2500 0.2500 0.0520(3) 0.0201(9) Uani 1 8 d S T P
P3 P 0.2500 0.2500 0.3365(10) 0.0057(19) Uani 1 8 d S T P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sn Sn -0.6537 1.4246 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
P3 Eu1 P3 88.71(17) . 9_556
P3 Eu1 P3 88.71(17) . 9_666
P3 Eu1 P3 177.4(3) 9_556 9_666
P3 Eu1 P3 88.71(17) . 9_566
P3 Eu1 P3 89.971(8) 9_556 9_566
P3 Eu1 P3 89.971(8) 9_666 9_566
P3 Eu1 P3 88.71(17) . 9_656
P3 Eu1 P3 89.971(8) 9_556 9_656
P3 Eu1 P3 89.971(9) 9_666 9_656
P3 Eu1 P3 177.4(3) 9_566 9_656
P3 Eu1 Sn2 180.0 . 1_556
P3 Eu1 Sn2 91.29(17) 9_556 1_556
P3 Eu1 Sn2 91.29(17) 9_666 1_556
P3 Eu1 Sn2 91.29(17) 9_566 1_556
P3 Eu1 Sn2 91.29(17) 9_656 1_556
P3 Eu1 Sn2 128.66(4) . 9_666
P3 Eu1 Sn2 142.63(18) 9_556 9_666
P3 Eu1 Sn2 39.94(17) 9_666 9_666
P3 Eu1 Sn2 90.80(11) 9_566 9_666
P3 Eu1 Sn2 90.80(11) 9_656 9_666
Sn2 Eu1 Sn2 51.34(4) 1_556 9_666
P3 Eu1 Sn2 128.66(4) . 9_566
P3 Eu1 Sn2 90.80(11) 9_556 9_566
P3 Eu1 Sn2 90.80(11) 9_666 9_566
P3 Eu1 Sn2 39.94(17) 9_566 9_566
P3 Eu1 Sn2 142.63(18) 9_656 9_566
Sn2 Eu1 Sn2 51.34(4) 1_556 9_566
Sn2 Eu1 Sn2 67.03(4) 9_666 9_566
P3 Eu1 Sn2 128.66(4) . 9_656
P3 Eu1 Sn2 90.80(11) 9_556 9_656
P3 Eu1 Sn2 90.80(11) 9_666 9_656
P3 Eu1 Sn2 142.63(18) 9_566 9_656
P3 Eu1 Sn2 39.94(17) 9_656 9_656
Sn2 Eu1 Sn2 51.34(4) 1_556 9_656
Sn2 Eu1 Sn2 67.03(4) 9_666 9_656
Sn2 Eu1 Sn2 102.69(8) 9_566 9_656
P3 Eu1 Sn2 128.66(4) . 9_556
P3 Eu1 Sn2 39.94(17) 9_556 9_556
P3 Eu1 Sn2 142.63(18) 9_666 9_556
P3 Eu1 Sn2 90.80(11) 9_566 9_556
P3 Eu1 Sn2 90.80(11) 9_656 9_556
Sn2 Eu1 Sn2 51.34(4) 1_556 9_556
Sn2 Eu1 Sn2 102.69(8) 9_666 9_556
Sn2 Eu1 Sn2 67.03(4) 9_566 9_556
Sn2 Eu1 Sn2 67.03(4) 9_656 9_556
P3 Eu1 Eu1 45.28(4) . 9_556
P3 Eu1 Eu1 43.43(16) 9_556 9_556
P3 Eu1 Eu1 134.00(19) 9_666 9_556
P3 Eu1 Eu1 89.09(12) 9_566 9_556
P3 Eu1 Eu1 89.09(12) 9_656 9_556
Sn2 Eu1 Eu1 134.72(4) 1_556 9_556
Sn2 Eu1 Eu1 173.94(6) 9_666 9_556
Sn2 Eu1 Eu1 116.07(2) 9_566 9_556
Sn2 Eu1 Eu1 116.07(2) 9_656 9_556
Sn2 Eu1 Eu1 83.37(4) 9_556 9_556
P3 Eu1 Eu1 45.28(4) . 9_656
P3 Eu1 Eu1 89.09(12) 9_556 9_656
P3 Eu1 Eu1 89.09(12) 9_666 9_656
P3 Eu1 Eu1 134.00(19) 9_566 9_656
P3 Eu1 Eu1 43.43(16) 9_656 9_656
Sn2 Eu1 Eu1 134.72(4) 1_556 9_656
Sn2 Eu1 Eu1 116.07(2) 9_666 9_656
Sn2 Eu1 Eu1 173.94(6) 9_566 9_656
Sn2 Eu1 Eu1 83.37(4) 9_656 9_656
Sn2 Eu1 Eu1 116.07(2) 9_556 9_656
Eu1 Eu1 Eu1 60.33(4) 9_556 9_656
P3 Sn2 Sn2 106.73(9) . 9
P3 Sn2 Sn2 106.73(9) . 9_665
Sn2 Sn2 Sn2 146.54(18) 9 9_665
P3 Sn2 Sn2 106.73(9) . 9_565
Sn2 Sn2 Sn2 85.25(5) 9 9_565
Sn2 Sn2 Sn2 85.25(5) 9_665 9_565
P3 Sn2 Sn2 106.73(9) . 9_655
Sn2 Sn2 Sn2 85.25(5) 9 9_655
Sn2 Sn2 Sn2 85.25(5) 9_665 9_655
Sn2 Sn2 Sn2 146.54(18) 9_565 9_655
P3 Sn2 Eu1 180.0 . 1_554
Sn2 Sn2 Eu1 73.27(9) 9 1_554
Sn2 Sn2 Eu1 73.27(9) 9_665 1_554
Sn2 Sn2 Eu1 73.27(9) 9_565 1_554
Sn2 Sn2 Eu1 73.27(9) 9_655 1_554
P3 Sn2 Eu1 51.34(4) . 9_666
Sn2 Sn2 Eu1 158.07(12) 9 9_666
Sn2 Sn2 Eu1 55.39(6) 9_665 9_666
Sn2 Sn2 Eu1 100.36(5) 9_565 9_666
Sn2 Sn2 Eu1 100.36(5) 9_655 9_666
Eu1 Sn2 Eu1 128.66(4) 1_554 9_666
P3 Sn2 Eu1 51.34(4) . 9_656
Sn2 Sn2 Eu1 100.36(5) 9 9_656
Sn2 Sn2 Eu1 100.36(5) 9_665 9_656
Sn2 Sn2 Eu1 158.07(12) 9_565 9_656
Sn2 Sn2 Eu1 55.39(6) 9_655 9_656
Eu1 Sn2 Eu1 128.66(4) 1_554 9_656
Eu1 Sn2 Eu1 67.03(4) 9_666 9_656
P3 Sn2 Eu1 51.34(4) . 9_566
Sn2 Sn2 Eu1 100.36(5) 9 9_566
Sn2 Sn2 Eu1 100.36(5) 9_665 9_566
Sn2 Sn2 Eu1 55.39(6) 9_565 9_566
Sn2 Sn2 Eu1 158.07(12) 9_655 9_566
Eu1 Sn2 Eu1 128.66(4) 1_554 9_566
Eu1 Sn2 Eu1 67.03(4) 9_666 9_566
Eu1 Sn2 Eu1 102.69(7) 9_656 9_566
P3 Sn2 Eu1 51.34(4) . 9_556
Sn2 Sn2 Eu1 55.39(6) 9 9_556
Sn2 Sn2 Eu1 158.07(12) 9_665 9_556
Sn2 Sn2 Eu1 100.36(5) 9_565 9_556
Sn2 Sn2 Eu1 100.36(5) 9_655 9_556
Eu1 Sn2 Eu1 128.66(4) 1_554 9_556
Eu1 Sn2 Eu1 102.69(7) 9_666 9_556
Eu1 Sn2 Eu1 67.03(4) 9_656 9_556
Eu1 Sn2 Eu1 67.03(4) 9_566 9_556
Sn2 P3 Eu1 180.0 . .
Sn2 P3 Eu1 88.71(17) . 9_556
Eu1 P3 Eu1 91.29(17) . 9_556
Sn2 P3 Eu1 88.71(17) . 9_666
Eu1 P3 Eu1 91.29(17) . 9_666
Eu1 P3 Eu1 177.4(3) 9_556 9_666
Sn2 P3 Eu1 88.71(17) . 9_656
Eu1 P3 Eu1 91.29(17) . 9_656
Eu1 P3 Eu1 89.971(8) 9_556 9_656
Eu1 P3 Eu1 89.971(8) 9_666 9_656
Sn2 P3 Eu1 88.71(17) . 9_566
Eu1 P3 Eu1 91.29(17) . 9_566
Eu1 P3 Eu1 89.971(8) 9_556 9_566
Eu1 P3 Eu1 89.971(8) 9_666 9_566
Eu1 P3 Eu1 177.4(3) 9_656 9_566
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Eu1 P3 2.890(8) .
Eu1 P3 2.9868(5) 9_556
Eu1 P3 2.9868(5) 9_666
Eu1 P3 2.9868(5) 9_566
Eu1 P3 2.9868(5) 9_656
Eu1 Sn2 3.286(3) 1_556
Eu1 Sn2 3.824(2) 9_666
Eu1 Sn2 3.824(2) 9_566
Eu1 Sn2 3.824(2) 9_656
Eu1 Sn2 3.824(2) 9_556
Eu1 Eu1 4.202(3) 9_556
Eu1 Eu1 4.202(3) 9_656
Sn2 P3 2.456(9) .
Sn2 Sn2 3.1180(15) 9
Sn2 Sn2 3.1180(15) 9_665
Sn2 Sn2 3.1180(15) 9_565
Sn2 Sn2 3.1180(15) 9_655
Sn2 Eu1 3.286(3) 1_554
Sn2 Eu1 3.824(2) 9_666
Sn2 Eu1 3.824(2) 9_656
Sn2 Eu1 3.824(2) 9_566
Sn2 Eu1 3.824(2) 9_556
P3 Eu1 2.9868(5) 9_556
P3 Eu1 2.9868(5) 9_666
P3 Eu1 2.9868(5) 9_656
P3 Eu1 2.9868(5) 9_566
